Open-framework zinc and cobalt phosphates synthesized by the tributylphosphate routeElectronic supplementary information (ESI) available: Tables S1?16: Atomic coordinates, equivalent isotropic displacement parameters and bond lengths and angles for compounds I?VII. See http://www.rsc.org/suppdata/jm/b3/b311529a/
Neeraj, S.; Rao, C. N. R.; Cheetham, Anthony K.; Journal of Materials Chemistry 14 (2004) 814–; doi:10.1039/b311529a

data_7204748
_publ_section_title
;
 Open-framework zinc and cobalt phosphates synthesized by the
 tributylphosphate routeElectronic supplementary information (ESI)
 available: Tables S1?16: Atomic coordinates, equivalent isotropic
 displacement parameters and bond lengths and angles for compounds
 I?VII. See http://www.rsc.org/suppdata/jm/b3/b311529a/
;
_journal_issue                   5
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              814
_journal_paper_doi               10.1039/b311529a
_journal_volume                  14
_journal_year                    2004
_chemical_formula_moiety         '[C4N2H12]3[Co2(OH)(HPO4)3]2'
_chemical_formula_sum            'C6 H21 Co2 N3 O13 P3'
_chemical_formula_weight         554.03
_chemical_name_common            'Cobalt Phosphate'
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 93.131(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.2743(18)
_cell_length_b                   23.030(6)
_cell_length_c                   9.873(2)
_cell_measurement_temperature    293(2)
_cell_volume                     1651.5(7)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.946
_diffrn_measured_fraction_theta_max 0.946
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0640
_diffrn_reflns_av_sigmaI/netI    0.0615
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            10083
_diffrn_reflns_theta_full        28.24
_diffrn_reflns_theta_max         28.24
_diffrn_reflns_theta_min         2.25
_exptl_absorpt_coefficient_mu    2.377
_exptl_crystal_density_diffrn    2.228
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1124
_refine_diff_density_max         1.253
_refine_diff_density_min         -0.943
_refine_diff_density_rms         0.178
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.030
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     243
_refine_ls_number_reflns         3857
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.030
_refine_ls_R_factor_all          0.0727
_refine_ls_R_factor_gt           0.0501
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0894P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1348
_refine_ls_wR_factor_ref         0.1464
_reflns_number_gt                2831
_reflns_number_total             3857
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b311529a.txt
_cod_data_source_block           COMPOUND_VI
_cod_original_cell_volume        1651.4(7)
_cod_database_code               7204748